distribution in green ceramics bodies via
zur Erlangung des akademischen Grades
genehmigt durch die
Fakultät (Ingenieurwissenschaftlicher Bereich)
der Martin-Luther-Universität Halle-Wittenberg
von Herrn Dipl.-Ing. Danail Donchev
geb. am 24.05.1974 in Kazanlak / Bulgarien
Dekan der Fakultät: Prof. Dr. habil. Altenbach
1. Prof. Dr. habil. Ulrich
2. Prof. Dr. König
18.08.05 Halle (Saale)urn:nbn:de:gbv:3-000010045
My grateful appreciation to my supervisor, Prof. Dr-Ing. habil. Joachim
Ulrich for his help, guidance and a continued encouragement, which not only
account for a major part of my knowledge but also strongly fuel my interest
in direction crystallization and ceramic materials as this thesis shows.
I would like to thank Prof. König for serving and helpful referring on my
I would also like to thank Prof. Rogendorf for serving as the Chairman of the
Ph.D. defense committee.
I am grateful to Martin-Luther-University Halle-Wittenberg, especially
Engineering Department, for admitting me as a graduate student in 2001. To
me, M.L.U. is a very special place, and I thank all those who contribute to and
are in stewardship of this unique and friendly environment.
I acknowledge the DFG Fellowship for providing financial support during my
I would like to thank Dr. L. Andresen, Dr. D. Koch and Prof. G. Grathwohl for
their hospitality during my visits to the Bremen University, where I learned
the techniques of Freeze-casting.
I would like to thank Dr. Diter Möring for his support, fruitful discussions
I would like to thank Dr. Jung-Woo Kim, Dr. Tero Tahti and Dr. Jun-Jun Lu,
you are all wonderful friends. I will always remember the many happy
occasions and what I learned from you.
I would like to thank all previous and present members of TVT group for
their help during my studying.
I must thank my dear wife Venelina who has supported me during the years.
Special thank to my two kids Simona and Pavlin for their obedience during
I thank my mother, father, sister and grandmother for their fortitude and
encouragements that helped build my character and stimulated my interest
in science since childhood.
Table of contents
1 Introduction 1
2 Technical background and theory 3
2.1 Nucleation 3
2.1.1 Homogeneous Nucleation 4
2.1.2 Heterogeneous Nucleation 6
2.1.3 Active Site Nucleation 8
2.2 Crystal growth 11
2.2.1 Theory of crystal growth 11
2.2.2 Crystal growth kinetics 13
2.3 Porosity and pore size distribution 14
2.3.1 Open, close, and total porosity 14
2.3.2 Pores characteristics 15
2.3.3 Methods and techniques for production of porous ceramics 16 2.3.4 Methods for characterizing porous ceramic materials 18
2.4 Freeze-casting. Bases and principles 20
2.4.1 Colloidal systems. Introduction 20
2.4.2 Freeze-casting 21
3. Materials and Experimental Setup 25
3.1 Materials 25
3.2 Experimental procedure and setup 26
4 Instrumentation 29
5 Results 30
5.1 Rheology 30
5.1.1 Density 30
5.1.2 Viscosity 32
5.2 Nucleation and Crystal growth 37
5.2.1 Nucleation 37
18.104.22.168 Roughness of the cooling plates 37
22.214.171.124 Contact angle 39
126.96.36.199 Surface tension of suspensions 42 188.8.131.52 Interfacial tension, suspensions-cooling plate 43
184.108.40.206 Nucleation kinetic 48 220.127.116.11 Determination of freezing and melting
18.104.22.168.1 Cooling curves 56
22.214.171.124.2 Melting points 57
5.2.2 Crystal growth rate 59
126.96.36.199 Influence on crystal growth rate in dependence of the volume fraction of solids
188.8.131.52 Influence on crystal growth rate in dependence on cooling plate materials and properties
184.108.40.206 Influence on crystal growth rate in dependence of moulding form materials and properties
5.3 Porosity and pore size distribution 66
5.3.1 Porosity 67
220.127.116.11 Porosity dependence of solids load content 67
18.104.22.168 Porosity dependence of freezing temperature 68 22.214.171.124 Porosity in dependence of cooling plate materials 70 126.96.36.199 Porosity in dependence of moulding form
5.3.2 Pore size distribution 72
188.8.131.52 Pore size distribution in dependence of solid load content
184.108.40.206 Pore size distribution in dependence of freezing temperature
220.127.116.11 Pore size distribution in dependence of cooling plate materials
18.104.22.168 Pore size distribution in dependence of moulding
6. Discussions 81
6.1 Discussions of rheological properties on the starting slurries and the dependence on porosity as well as the pore size distribution
6.2 Discussions on contact angle, interfacial tension and nucleation kinetics
7. Conclusions 100
8. Zusammenfassung 102
9. List of Symbols 103
10. Appendix 107
Porous ceramics have attracted very high interests of the scientific and industrial parties during the past two decades. This is especially true for forming techniques that offer great flexibility and trustworthiness. The efforts have been invested because of the necessarily of porous ceramic materials as filters, dust collectors, absorbers, dielectric resonators, thermal insulation, bioreactors, bone replacement, hot gas collectors, automobile engine components. There could be named many other applications.
Several methods have been tried to produce ceramic materials with an open pore structure such as injection moulding, acid leaching etc. One of the most common ways is to add to ceramic powder an organic material that is burning out during sintering. However, the problem with these methods is, that they are harmful to the environment, and the pore structure cannot be controlled.
This thesis concentrates on the properties of highly porous ceramics and one of the most promising methods to create them. Microstructural features are the most determining factoring of that technology. It is the freeze-casting method that has been employed. The products, the ceramic green bodies, produced by this method are of high porosity and uniformity concerning size and morphologies as well as pore structure. Specific characteristics that distinguish the freeze-casting route from conventional fabrication processes are to offer great possibilities to control porosity and pore size distribution and its simplicity. Furthermore, this method is applicable to many types of ceramics. However, on this technology is rarely reported concerning the preparation of macroporous ceramics.
Freeze casting is based on phase separation during freezing. It requires preparation of aqueous ceramic slurry which is poured into a mould, and then been frozen. After a complete freezing the samples are subject to ice sublimation and water removing. The pore structure, morphology and size, which are gained and remain, are the negative image of the ice crystals. A good knowledge and control of the
crystallization process is, therefore, needed.
The aim of the presented work is to achieve simple, systematic and effective ways to control porosity and the pore size distribution. Therefore, this work aims for an in depth understanding of the factors and parameters effecting ice crystallization.
The experimental work is divided in to two major parts. The first part deals with the factors affecting and controlling nucleation, are furthermore, ice crystal growth. Solid load content and its consequence on the crystallization process are studied. Factors such as cooling plate and moulding form materials and their physical properties have been exanimate, too. To attain a deeper insight in real structures, the main objective of this thesis is to evaluate experimentally the characteristics of the obtained pores such as porosity, pore morphology and pore size distribution in dependence of the crystallization process. These results are given in the second part. Since suspension characteristics, especially, solid load contents are known to be very important in practical situations and have been found to be one of the major parameter to manage porosity and pore size distribution, they have also been studied and discussed
In this thesis are presented results of successful attempts to develop porous ceramic products with well controlled of porosity and pore size distribution.
2 Theoretical backgrounds
When a liquid is cooled, there exists a temperature at which it turns to solid. The first formed solid embryos or nuclei, which can only be a few nanometres in size, appear when the system is supersaturated [Jon02]. Supersaturated solutions exhibit a metastable zone in which all crystallization processes take place. Even when a solution is supersaturated nucleation do not start always spontaneously. Whenever the upper limit of the metastable zone of the supersaturation is reached nucleation will occur spontaneously. This happens when the system reaches the metastable limit ∂2G/∂x2 =0 [Mye02].
Frequently nucleation can be promoted by agitation, shearing action, crystal breakage or abrasion, and pressure changes [Mul01].
There are different kinds of nucleation processes:
If a solution contains no foreign particles or crystals of it’s own type, nucleus can only be formed by homogeneous nucleation. If foreign surfaces (particles) are present in the system, it is possible for a liquid to form on those surfaces nuclei at less
supersaturation compared to the case of homogeneous nucleation. This process is called heterogeneous nucleation [Mer01]. It has been observed that nuclei occur even at very low supersaturations. This is the case when crystals of the same material exist and act as attrition agents or seed crystals [Mul01]. Such nuclei are known as secondary nuclei.
Fig. 2-1: Mechanisms of nucleation, according to [Mul01]
(induced by crystals)
(induced by foreign
(induced by crystals)
(induced by foreign
Figure 2-2: Concentration against temperature for several types of nucleation processes [Mer01]
2.1.1 Homogeneous Nucleation
Exactly how stable nuclei and crystals are formed within a homogeneous fluid is not known with any degree of certainty. The theories for homogeneous nucleation processes are communicated by Becker and Döring [Bec35], Volmer [Vol39] and Gibbs [Gib48]. The classical theories of nucleation suppose that the clusters are formed by an additional mechanism until the critical size is reached.
A+A=A2 A2+A=A3 ……. An+A=An+1 (2.1)
The classical theory of nucleation is based on a condensation of a vapour to liquid, and can be extended to crystallization from melts and solutions.
The change of the free energies associated with the process of homogeneous nucleation may be considered as follows:
v V S G r r G G G=∆ +∆ = + ∆ ∆ 2 3 3 4 4π σ π (2.2)
where ∆GS is the excess free energy between the surface of the particle and the
bulk. ∆GV is excess free energy between a very large particle and the solute in
C*=f (T) Metastable zone width for nucleation Secondary Primary heterogeneous Primary homogeneous
solution. For homogeneous nucleation the volume free energy for supercooling can be expressed by: * T T H Gv = ∆ f∆ ∆ (2.3)
The two terms on the right- hand side of equation (2.2) have an opposite effect on the system and they depend differently on the radius of the nucleus r. Therefore the free energy of formation ∆Gpasses through a maximum value ∆Gcryt, which
corresponds, to the nucleus critical size. From Fig. 2-3 it can be seen that ∆GS is a
positive quantity, proportional to r2. ∆G
V is a negative quantity proportional to r3.
Fig. 2-3: Free energy diagram for nucleation explaining the existence of a critical nucleus (according to [Mul01])
With respect to r the critical size for a spherical nucleus can be obtained from equation 2.2 as follows: 0 4 8 + 2∆ = = ∆ v G r r dr G d π σ π (2.4) 0 F re e E n e rg y ∆ G +ve -ve rc ∆Gcryt ∆GV ∆GS Size of nucleus, r 0 F re e E n e rg y ∆ G +ve -ve rc ∆Gcryt ∆GV ∆GS Size of nucleus, r
or v c G r ∆ − = 2σ (2.5) The rc represents the minimal size of a nucleus which needs to be gained before the
new phase is formed. If the cluster size is smaller than the critical size they can easily be dissolved back in the liquid or evaporate. From Fig. 2-3 it can be seen that nuclei with sizes larger rc will reduce the energy necessary to get a stable nucleus which
can continuously grow into crystals [MUL01]. Combining the equations 2.2 and 2.5 it leads to:
3 4 ) ( 3 16 2 2 3 c v cryt r G G πσ = πσ ∆ = ∆ (2.6)
The nucleation rate can be expressed as follows:
⎥ ⎦ ⎤ ⎢ ⎣ ⎡ − = 3 3 3 22 ) (ln 3 16 exp S T k A J πσ υ (2.7)
The nucleation process is strongly depending on the interfacial tension. This is one of the most difficult parameters concerning the measurements, when trying to calculate nuclei critical size.
There are a lot of theories [Kash00], [Mer01], [Mul01], trying to explain physically and mathematically the mechanism for homogeneous and heterogeneous nucleation but even with lot of research performance there is no general theory, which can explain and calculate experimental data in good agreement.
2.1.2 Heterogeneous Nucleation
It has been known for many years that different heterogeneities, motes, inclusions, etc. can encourage phase transformations (by reducing formation energies), mainly condensation and crystallization.
Nucleation in heterogeneous systems normally occurs at lower supersaturations compared with homogeneous nucleation (see Fig. 2-2). Therefore a correction factor is needed which, must be less than a unit and can be explained as follows:
hom G f Ghet = ∆ ∆ (2.8) where 4 ) cos 1 )( cos 2 ( + θ − θ 2 = f (2.9)
where θ is the contact angle between liquid and solid surface. The contact angle θ is determined by Young’s relation [Youn55].
cl cs sl σ σ σ θ = − cos (2.10)
where σsl is the solid-liquid interfacial tension, σcs is crystal-solid interfacial tension
and σcl crystal-liquid interfacial tension (see Fig. 2-4).
Fig. 2-4: Contact angle and interfacial tension
It is assumed that a free liquid drop automatically takes the shape that minimizes the free energy of the entire system. A surface with cluster contact angle of zero is known as wetting while a surface with cluster contact of more than 90° is known as non-wetting [Ada97]. When the contact angle is between 0° to 90° a system is known as partially wetting. A surface will also be known as hydrophilic if liquid wets the surface and as hydrophobic if a water cluster has a contact angle greater than 30° on the surface. In general, there appears to be only a limited number of places at which nuclei can form. Nuclei are always formed on a surface [Gar55] (see Fig. 2-5).
Substrate New phase σcl σcs σsl Radius, r Parent phase θ Substrate New phase σcl σcs σsl Radius, r Parent phase θ
Fig. 2-5: Heterogeneous nucleation occurs on foreign surfaces or interfaces
2.1.3 Active Site Nucleation
If geometric or chemical inhomogeneities are added to the liquid, nucleation may occur on the surface of these inhomogeneities at lower supersaturations. In this case the inhomogeneities are known as active sites.
Formation of stabile clusters on inhomogeneities or active sites has recently received growing experimental and theoretical interest. Several authors have published
theoretical and experimental work[Gor01, Gor82, Fle58, Fle62, For03, Lee98, Meg02, Pad01, Smo87, Ylee98]. Although many theories have been developed as shown in Fig. 2-5 the cluster formation can occur on bubbles or on foreign particles. Therefore a cluster on a special convex surface as shown in Fig. 2-6 the volume is given by:
) (cos 3 4 ) (cos 3 4π 3 ψ π 3 φ g R g r V = − (2.11)
The critical free energy of the cluster is given by (see [Fle58]) ) , ( ) ( 3 16 2 3 * f m x G G v ∆ = πσ (2.12) where
⎟ ⎠ ⎞ ⎜ ⎝ ⎛ − − + ⎥ ⎥ ⎦ ⎤ ⎢ ⎢ ⎣ ⎡ ⎟ ⎠ ⎞ ⎜ ⎝ ⎛ − + ⎟ ⎠ ⎞ ⎜ ⎝ ⎛ − − + ⎟ ⎠ ⎞ ⎜ ⎝ ⎛ − + =1 1 2 3 3 1 2 2 3 3 3 k m x mx k m x k m x x k mx ) x , m ( f (2.13) with,
)2 1 2 2 1 x mx k= + − , m=cosθ, * r R
x= where r* is given by Eq. 2.5.
Fig. 2-6: Cluster formation on spherically convex surface (see [Fle58])
Fletcher [Fle62] observed the conditions, which are required for nucleation in a conical cavity at a spherical particle. He assumed that ice completely filled the cavity and that the surface curvature of the vapour-ice interface is the same as that of the curved surface (see Fig. 2-7).
Fig. 2-7: A spherical particle of radius R and surface parameter m containing a conical cavity of semi-angle f and surface area αR2 (see [Fle62])
Fletcher gave the nucleation rate per particle as
)J R J ≈4π 2 oexp− cryt/ (2.14) with
)σ G v cryt − − ∆ = , 1 3 16 2 2 3 (2.15)
where αR² is the surface area of cavity (see Fig. 2-7).
Contrasting with Fletcher, Gorbunov and Kakutina [Gor82] take different stages into account during the formation of stabile clusters on active sites [see Fig. 2-8].
Fig. 2-8: Stages of cluster growth on an active site
For the first stage (Fig. 2-8a) the free energy of a cluster is given as:
)lv lv V S S G V G1 = ∆ + σ + −σcosθ (2.16)
After the cluster reaches the active site boundaries (Fig. 2-8b), the contact angle changed from Θa to Θ. Therefore the energy in this stage is given as:
2 =V∆GV +Slv +Sa −
In the third stage (Fig. 2-8c) cluster grow beyond active sites and the contact angle is changed from Θto Θ0.
3 =V∆GV +Slvσ +Slv −σcosθo +Sa −σcosθa +σcosθ
G (2.18) r r r ra Θa Θ Θ0
cr r r ra Θa Θ Θ0
A lot of efforts have been carried out to investigate nucleation on active sites. Different models and theories have been developed but the nucleation process is very complex and has not been well understood up to now.
2.2 Crystal growth
2.2.1 Theory of crystal growth
After the nucleus reaches the critical size it begins to grow by adding and
incorporating of units. This stage of the crystallization process is known as crystal growth [Mye01, Mul01]. Nucleation and crystal growth are the primary particle formation processes during crystallization and have large effects in determining product crystal size distributions [Jon02].
Crystal’s growth and habit have for long been in the centre of the interest of scientists, but are still not well understood up to now.
Many theories dealing with crystal growth have been developed. But none has succeeded to be generalized for the growth mechanism. This is due to the fact that many varieties of mechanisms needs to be considered before growth units, from the solution, reach and incorporated in to the crystal surface.
According to Garside [Gar90] there are three main ways to express the growth rate of a crystals or population of crystals:
1. Face growth rate, vhkl. This is the rate of advance of the crystallographic
face, measured perpendicular to the face. It means the individual crystal face needs to be observed and measured. The illustration of these theories can be taken from Burton, Cabrera, Frank (BCF model) [Bur51], or “birth and spread” (BS) model, purposed by O’Hara and Reid [Oha73].
2. Overall mass growth rate, best expressed as the total mass flux to the crystal surface, RG. This is the growth rate over the whole crystal.
dt dM A R C C G . 1 = (2.19)
are known, RG can be related to the different values of vhkl by the expression:
∑= hkl hkl c c G v A A R ρ * (2.20)
The overall mass growth rate is mainly used for calculations in batch systems.
3. Overall linear growth rate, which is defined as the time rate of change of a characteristic dimension, L, of the crystal.
The overall linear growth rate is widely used in population balance theory for calculating continuous and batch crystallizers.
Reviews on crystal growth theories can be found e.g. in the works of Ohara and Reid [Oha73], Strickland-Constable [Str68], Nyvlt et al. [Nyv85] and [Shö92]. Table 2.2.1 provides a summary of these growth models.
Table 2.2.1: Growth rate models (according to [Oha73])
Two-dimensional growth models
]⎟ ⎟ ⎠ ⎞ ⎜ ⎜ ⎝ ⎛ − ⎟⎟ ⎠ ⎞ ⎜⎜ ⎝ ⎛ = S ln ) C C ln( K exp C C d D C * C m AB PN π ν ∆ υ 2 3 2 3 With C M~ n ρ ν = & B+S model ⎟⎟ ⎠ ⎞ ⎜ ⎜ ⎝ ⎛ ∆ ⎟ ⎠ ⎞ ⎜ ⎝ ⎛ ∆ = + + + C C T K C C KB S B S S B * ' 6 5 * exp υ
BCF surface diffusion model
BCF Model ⎟⎟ ⎠ ⎞ ⎜ ⎜ ⎝ ⎛ ⋅ ⎟ ⎠ ⎞ ⎜ ⎝ ⎛ = C C T K h tan C C T K * ' ' BCF 2 * BCF BCF ∆ ∆ υ
Diffusion layer model Only convection and diffusion n& = kd(C − Ci )
Only surface integration n& = kr(Ci −C*)
with kr =kr0exp
), Elimination of Ci r d r k n C k n ⎟⎟ ⎠ ⎞ ⎜⎜ ⎝ ⎛ − = & & ∆ Special case r = 1 r d K 1 k 1 C n + = ∆ & Special case r = 2 r 3 d 2 r 4 d r 2 d d k C k k 4 k k 2 k C k n& = ∆ + − + ∆
2.2.2 Crystal growth kinetics
Design of industrial crystallizers and crystallization processes is based on
calculations of crystal growth kinetics. Such calculations can be obtained if the data on crystal growth kinetics are available.
One of the main parameters for controlling the crystal growth is supersaturation, which can be expressed in a simplified form as follows:
* C C C = C −
From here the equations for linear and mass growth rate can be rewritten: g g C k G= ∆ (2.23) and g g G K C R = ∆ (2.24)
The constants Kg and kg are related to each other through the expression:
g g k K ρ β λ 3 = (2.25)
Both constants Kg and kg are temperature dependentand can be fitted to the
Arrhenius equation, which can be rewritten, for growth rates, as a function of temperature as follows: ) RT / E exp( A kg = − G (2.26)
The activation energy can be used to obtain information of whether the rate-controlling step is diffusion or surface integration [Nỳv85]. Therefore the equation (2.23) can be written as:
g G /RT) C E exp( A G= − ∆ (2.27)
In this equation both parameters temperature and supersaturation are taken into account.
The techniques used to measure crystal growth rates can be divided into two main groups. In the first group are methods using data obtained from single crystals and in the second group are methods using suspension of crystals. Reviews and
information about crystal growth rate measurements and techniques can be found in [Gar90], [Mul01] [Nỳv85] and [Ulr89]
2.3 Porosity and pore size distribution
2.3.1 Open, close, and total porosity
Many solids and powder materials, natural or manufactured contain a certain volume of voids and empty spaces. This is distributed within the solid form of pores, cavities and cracks of various shapes and sizes. The total sum of this voids volume is called porosity. Porosity is defined as the ratio of the void volume Vv to the total volume Vtot
of the specimen. tot V V V = ε (2.28)
¾ Total porosity, this is the sum of open and closed porosity, Eq. 2.29. ¾ Open or effective porosity, which may be defined continuous, channels
involving connecting the interior of the specimen with the surrounding gas or liquid phase. Effective porosity is less than total porosity.
¾ Closed porosity contains pores, which are completely isolated from the external surface, not allowing access of external liquids or gaseous phases (see Fig. 2-9), [Rav97, Som00]. This closed porosity is impossible to be measured directly. Data about it can only be gained with measurements of the apparent density.
The sum of effective and closed porosity gives the total porosity.
tot ε ε
ε = + (2.29)
Closed porosity has a great influence on physical parameters like density, mechanical or thermal properties. Open pores are connected with the external specimen surface and therefore allowing liquids or gases to flow through or into the porous article. Open pores can be further divided in dead-end or interconnected pores. Dead-end pores have access to external specimen surface at one of the ends while the other one is closed. Interconnected pores have an access with external surface with the both ends or one of the ends is connected with other pores.
The type and nature of porosity in natural materials depend on their genesis while in synthetic materials it depends on their manufacturing and generally it can be
2.3.2 Pores characteristics
The characterization of solids in terms of porosity can be determined by the parameters of the pores:
Pore size is the dimension, which classified the pores up to their sizes (see Fig. 2-10) to micropores, mesopores and macropores. Several techniques are on hand to examine pores depending on their size and nature. They will be discussed in section 2.3.3.
Specific pore volume and porosity: The internal void space in a porous material can be measured. It is generally expressed as a void volume (in cc or ml) referred to the mass unit (g).
Pore size distribution: The pore size distribution represents the pore volume in function of pore size and commonly is given as percentage or a derivative
Percentage porosity: Corresponding to the ratio between the total pore volume and the external sample volume.
Specific surface area: This is the total surface area of the sample, which is in contact with the external environment. This parameter is mainly dependable to the pore size and the pore volume. The smaller the pore size is the higher is the surface area [Por02].
Fig. 2-9: Structure of open and closed pores
2.3.3 Methods and techniques for production of porous ceramics
Methods and techniques of creating porosity depend on the wanted porosity or on the techniques and devices to obtain it. More information about different techniques can be found e.g. in the following books Segal [Seg89] and Liu [Liu96, Liu97].
All fabrication techniques and methods lead to a variety of microstructure. As discussed in the previous section most of the macro properties such as density, thermal expansion, electrical conductivity, melting points, Young’s modulus and thermal expansion are to a large extend microstructural dependent [Bar03]. However, all microstructural properties are in consequence based on used manufacturing procedure and the starting materials characteristics.
Closed inaccessible pores Accessible pores
SolidClosed inaccessible pores Accessible pores
Methods and techniques used to obtain porosity may be categorized as follows [Liu97]:
¾ Porosity formers by gas development give rise to a reaction of chemical scission of the constituting molecules activated by heating, with development of one or more gaseous components. Among them are the classical CaCO3,
NH4NO3, (NH4)2CO3, and other can be taken into account. Developing of gas
involves its outlet along radial directions in respect to the site of emission. Since the sites of emission are distributed homogeneously, the obtained porosity is distributed randomly. The functionality of such agents may be expressed only if the temperature of chemical scission occurs just slightly below the one at which the sintering begins, a step in which the small channels are created as a result of gas outlet can be maintained for the stiffening due to sintering for the join of the grains.
¾ Volume preserver agents involve substances like NaCl, grains of sugar, etc. which are able to resist chemically the increase of temperature at least until the start of ceramic sintering. Such agents preserve the volume, which they occupied. In this way the body on the way to be ceramized actuate remarkably well a sufficient number of intergranular linking’s. After the sintering, when the body becomes ceramics cold, the preserver agents are taken away by simple immersion in a liquid medium (mostly H2O) in which they are soluble. The
volume occupied by the disappeared agents is set free, so obtaining the desired porosity.
¾ Thermounstable porosity formers are agents constituted by organic substances, which disappear during heating, leaving empty volume, which they occupied. Their disappearance must happen just below the consolidation temperature or, at least, over specific threshold temperatures. The formation of gas, if any, along the formed and preserved meanders contributes to the preservation of the porous volume. The nature of the involved processes of disappearance can be chemical and/or physical
• sublimation (e.g. naphthalene, camphor, etc.)
¾ Agents for replamineform process are porous substances, generally natural, the porous structure of which is considered for serial reproduction. The process consists in reproducing in negative or in positive (terms taken from photographs) the porous network of such porous substances. These are generally natural (e.g. porites, corals, Madrepores, etc.). If the starting material is easily dissolvable chemically with specific substances, as in the case of acids for the calcium phosphates of the natural corals, its natural porosity is filled with substances not affectible by them.
¾ Agents at cryoscopic action are liquids at very low temperature. These are used in particular to obtain porous granules. The process that requires them consists in plunging spheroidal bodies constituted by polymeric slurry of the starting powder into liquid nitrogen. The immersion of granulates into the freezing liquid produce fast decreases of their temperature with the consequence of the strong shrinkage of the volume of each granulate. This leads to the formation of microcracks, which the liquid nitrogen penetrates. The later becomes warm at contact with the warmer granule until overcoming the boiling temperature of nitrogen, becoming vapor with an expansion of volume.
2.3.4 Methods for characterizing porous ceramic materials
Many techniques have been developed for characterizing porous materials. Here can be noted methods such as gas adsorption, fluid penetration, NMR, ultrasonic
technique or other. The most popular and widely used methods are the gas adsorption and mercury intrusion porosimetry. To characterize mesopores and surface area the Brunauer, Emmett and Teller (BET) method is applied, and for macropores mercury porosimetry. Any condensable vapor can be used for BET. For this purpose the vapor molecules should be small and approximately spherical. Mainly liquid nitrogen is used. The measurement is based on the adsorption isotherms. For more details see [Bru44]. In this study mercury porosimetry will be used. This method is based on the physical properties of mercury. It is interacting with most of the solids as non-wetting liquid (contact angle, greater then 140°) and having a surface tension over 480dyne/cm [Was22, Por02]. This high surface tension
Micropores Mesopores Macropores
Gas adsorption (BET) Pore size
Micropores Mesopores Macropores
Gas adsorption (BET)
Fig. 2-10: Pore sizes and methods for their characterization
can be passed by applying external pressure. This external pressure is needed for the mercury to penetrate into small pores. Under this conditions the pore radius in which the mercury intrudes at a given external pressure can be calculated by the Washburn equation: e m m p P cos r = 2σ θ (2.31)
where θm is the contact angle between mercury and measured solid, Pe is the
external pressure, rp is the pore radius and σm is mercury surface tension. This
equation is applicable for cylindrical pores. For pores with other shapes a shape factor for corrections should be taken into account.
In this study a Mercury intrusion Porosimeter serial Pascal 140+440 is used. The sample is placed in a special holder (dilatometer) with known volume and put forward to vacuum. After an indispensable vacuum level is reached mercury is droped in the holder. So the volume of the macropores of the sample can be found, with respect to the large cavities, which can be filled by mercury at low pressure. The porosity of the sample is defined as the ratio between the samples voids volumes (inter and intra porosity) and its external volume [Por02].
[ ]100 1 % max BD V ρ ε = (2.32)
The apparent density is defined as the density of the sample referred to the real sample volume. The apparent density is very close to the real density (or true density) in the following cases:
• The sample is not collapsed by the high pressure
• The sample has no pores smaller than the mercury porosimetry lower limits The apparent density can be calculated as follows:
max ) 1 ( 1 V BD AD = ρ − ρ (2.33)
where ρAD is the apparent density, ρBD is the bulk density and Vmax is the total mercury
penetrated into the sample at the end of measurements referred to the sample mass (cumulative volume) and can be calculated as follows:
m c S
Vmax = (2.34)
where Vc is the cumulative volume and Sm is the sample mass. 2.4 Freeze-casting. Bases and principles
2.4.1 Colloidal systems. Introduction
The colloidal systems are defined as comprising a disperse phase with at least one dimension between 1nm and 1 µm in a dispersion medium [Seg89]. Examples of such a systems can be found in Tab 2.4.
One of the most important attributes of all colloidal systems is that the contact area between the phases is very large, and interparticle forces strongly influences the system behaviour.
Ceramics have been produced by different colloidal routs and techniques for several millennia. But in the last decades the research has been mainly focused on so-called “clay- based” systems. Colloidal processing offers a great potential for producing thin ceramic films and bulk forms through careful control of initial suspension “structure” and its evolution during fabrication [Lew00]. Five steps are involved for this purpose:
9 Powder synthesis 9 Suspension preparation
9 Removal of the solvent phase
9 Densification to produce the final microstructure required for optimal performance
Table 2.4 Classification of colloidal systems [Seg89]
System Disperse phase Dispersion medium
Dispersion (Sol) Solid Liquid
Emulsion Liquid Liquid
Solid emulsion Liquid Solid
Fog, mist or aerosol (of Liquid Gas
Smoke or aerosol (of Solid Gas
Alloy, solid suspension Solid Solid
The forces responsible for the colloid systems stability and interparticle potential can be summarized in the follow equation:
structural steric elect vdW Total F F F F F = + + + (2.35)
where FvdW is the attractive potential energy due to long-range van der Waals
interactions between particles, Felect the repulsive potential energy resulting from
electrostatic interactions between like-charged particle surfaces, Fsteric the repulsive
potential energy resulting from steric interactions between particle surfaces coated with adsorbed polymeric species, and Fstructural the potential energy resulting from the
presence of nonadsorbed species in solution that may either increase or decrease suspension stability.
More information and very deep investigation on colloidal processing of ceramics and sol-gel science and technology can be found e.g. by Lewis [Lew00], Segal [Seg89], Sigmund et al. [Sig00] and Lopez et al. [Lop03].
Colloidal processing techniques are typically used in complex-shape forming for ceramics. Colloidal processing contains methods such as slip casting, injection moulding [Nov92], gelcasting, [Mor99, Oma91, You91] and freeze- casting [Don04,
Jon00, Koc03, Sof01]. Among these colloidal processing techniques, freeze-casting is one of the simplest techniques.
First Smith-Johannsen [Smi61] reported a method for producing metallic and ceramic bodies by using freeze sensitive colloidal silica. Furthermore, Mahler [Mah78] and Mahler and Bechtold [Mah80] upgraded the existing method and used it for the production of Silica fibbers. A lot of investigations have been done in the past decade observing operating conditions [Don03, Don04, Don04a, Koc03], sintering [Fuk01, Sta98] and the effect of additives [Sof01] on the microstructure of produced
specimens by the freeze-casting route.
Freeze- casting is a technique, which takes ceramic slurries into a form of a
nonporous mould. The ceramic slurries containing freeze sensitive liquids (water or silica-sol), which can be frozen under extremely cold temperatures followed by demolding and liquid phase removal by sublimation. Polymerization occurs because of the concentration of silica particles within the interspaces between ice crystals [And03]. The polymerization process is schematically exposed in Fig. 2-11.
SolpH 7-10, salt conventional hydrogel freeze gelation
GelSi OH OH
OH Dimer Oligomer Particles
1 nm 5 nm 10 nm
SolpH 7-10, salt conventional hydrogel freeze gelation
GelSi OH OH
OH Dimer Oligomer Particles
Fig. 2-11: Polymerization process for Silica-Sol (Adopted from Andresen et al. [And03])
The important steps of the freeze- casting process are graphically shown in Fig. 2-12. The freeze-casting technique is based on a phase separation as a pore forming principle of aqueous suspensions with simultaneous growth for the ice crystals in one direction (see Fig. 2-13). After a complete freezing the samples are warmed to melt
Fig. 2-12: Flow chart of the freeze-casting process
or sublimate the ice crystals and then to dry the sample. The freezing agent acts temporary as binder. The result is a formation of rigid bodies [Sof01]. Therefore no binder agents are needed.
After drying the formed green body has a relatively high degree of overall porosity, where the pores reproducing the morphology and dimensions of the ice crystals formed during the freezing process [Sta98]. The pores are the negative images of the ice crystals. A control of pore size, shape and morphology of the ice crystals can be achieved by controlling nucleation and growth rate of the ice during the freezing [Don04, Don04a] and dependence of solid load content (filler) amount. Removing of the liquid phase by sublimation minimizes the possibility of stresses, which can occur due to the drying process [Lau92].
The freeze- casting route has many advantages such as a fast manufacturing cycle, no drying cracks, essentially zero-shrinkage [Sta98] and no troublesome binder burnout process [Ara04]. Also one of the advantageous of the freeze- casting process is a preparation of a highly concentrated suspensions [Hua01,Sta98]. Such a great additions of solid loads (over 70wt.%) can be a good enhancement of mechanical and thermal properties.
Alumina powder Silica-Sol Mixing of components Casting into the mould Freezing Drying Sintering Alumina powder Silica-Sol Mixing of components Casting into the mould Freezing Drying Sintering
Fig. 2-13: Phase separation of water and solid particles during freezing (Adopted from [Don04a]) Water Ice Al2O3 Al2O3 SiO2 Water Ice Al2O3 Al2O3 SiO2
3. Materials and Experimental Setup
As aqueous sol in this study Nyacol 1440, (EKA-Chemicals, Sweden) with 17 vol.% SiO2 suspended in water has been used, with a particle size d50=14nm and alumina
powder (99,99 wt.% Al2O3, CT 3000 SG, Alcoa, Germany) having an average particle
size of 700 nm and a surface area of 10,4 m²/g. Suspensions were prepared by mixing of known amount of dry powder (Al2O3) with silica sol to obtain the desired
volume fraction. The components were mixed by stirring and prepared at different solid loads in order to investigate the effect of the solid load content on the overall porosity and pore size distribution (see Fig. 3-1). After the alumina powder was added to the silica-sol the slurries were treated with an ultrasonic buster (Sonoplus HD220, Bandelin electronics, Germany) for about 5 min to prevent uncontrolled agglomerates formation and high densities zones. As dispersing agent Polyacrylic acid (35 wt.% solution in water Mw~100,000, Aldrich Chemicals Company Inc., Milwaukee, USA) has been used influencing the electrostatic stability of the suspensions and the surface charge of the particles.
H2O 0 10 20 30 40 50 60 70 80 90 100 SiO2 0 10 20 30 40 50 60 70 80 90 100 Al2O3 100 90 80 70 60 50 40 30 20 10 0
3.2 Experimental procedure and setup
The suspensions were poured into the polyethylene or glass moulding form, which were subsequently frozen from the bottom to the top (see Fig.3-2). A cooling device in which the temperature was controlled by a thermostatic bath provided the cooling from the bottom face. The top of the moulding form was always open, so the upper face of the suspensions was exposed to ambient conditions and a temperature gradient between the faces was generate. Therefore the ice crystals formed due to the freezing were encouraged to grow only in vertical direction. Different freezing temperatures have been utilized in order to examine closely ice crystals growth. The growth of ice crystals was observed using a CCD camera and a microscope. A connection of the camera to a computer allows getting on-line pictures for the
calculation of the linear ice growth rate. While freezing the phase separations occurs. The water forms during freezing ice crystals, which compact surrounding solid
particles (see Fig. 2-13). When the freezing begins and phase separation occurs columns of formed ice piled up between the surrounding ceramic particles. After complete freezing the samples were removed from the cooling device. Melting of the ice and then evaporation of the water was allowed to occur in the dryer for 24 hours.
Fig. 3-2: Experimental setup
The moulding forms, which have been used, had always the same dimensions, diameter 2cm and height of 5cm. To observe the influence of material properties
Flow direction Mixing of components Computer Cooling cell Cooling liquid Microscope and CCD camera Molding form Cooling plate Flow direction Mixing of components Computer Cooling cell Cooling liquid Microscope and CCD camera Molding form Cooling plate
respectively interfacial energies on nucleation and ice crystals growth different materials (glass and polyethylene) for the moulding form have been used. Furthermore, different shapes of the moulding forms have been examined. The second experimental setup is called “diffusion chamber” and consists of two reservoirs and five steel disks (see Fig. 3-3). Each disk has a thickness of 8mm and is insulated from the others and the reservoirs by teflon gaskets (see Fig. 3-4). Every teflon gasket has a thickness of 2mm.
Fig. 3-3: Diffusion cell (Adopted from [Neu95])
The disks, teflon gaskets and the bottom reservoir are fixed by a swivelling on an axle. Through the disks and the teflon gaskets 3 openings with a diameter of 1,5 cm are available. The upper reservoir was constructed that way that it allows to be removed. On this way the suspensions to be investigated can be mould into the disks openings. All the disks are routable against each other by 30°. By rotating of the disks the samples placed into the openings can be separated into different sections. All sections represent a part of the moulding form. The teflon gaskets are fixed on one of the disks so that the sections can be completely locked from each other.
Fig. 3-3: Schematic of diffusion cell
Cooling liquid Cooling liquid Flow direction Flow direction Flow direction Flow direction Teflon gasket Steel plate Opening
Cooling liquid Cooling liquid Flow direction Flow direction Flow direction Flow direction Teflon gasket Steel plate Opening
The top and the bottom reservoirs are double- jacked. By the connection with thermostats different temperature gradients can be applied. Even a freezing procedure of the samples from both sides is possible.
ViscoTester 550 (VT550 DIN/ISO Cylinder Package, HAAKE) rotational viscosimeter was used to investigate the suspensions viscosity. Suspensions density
measurements have been carried out by using Density/ Specific Gravity/
Concentration Meter - DMA 4500 (Anton Paar, Switzerland). The cooling plates roughness measurements were done using Perthometer S3P (Mahr, Göttingen, Germany). Optical Stereo Microscope Stemi 2000- C (Zeiss, Germany) was used to observe samples microstructural evolution and measurements for crystal growth. Ceramic particle surface and cooling plates microstructure have been observed with ESEM, Model XL30ESEM-FEG, XL Series (Philips). The contact angle
measurements were made using an Optical Contact Angle Measuring System OCA 20 (Krüss, Germany). Drop Shape Analysis System G10/DSA10 (Krüss, Germany) was used for determining surface energies of used suspensions. Thermostats FP 50 and FP 81 from Julabo (Julabo, Germany) were used for controlling of temperature and temperature gradients on cooling and diffusion cells. The measurements on overall porosity and pore size distribution were carried out by using system of mercury intrusion porosimeters Pascal 140 (low pressure) and Pascal 440 (high pressure), from Porotec, Germany. All samples have been dried, after freezing in a convection oven (AX60, Carbolite, Germany). Using DSC 12E Device from Mettler Toledo has done DSC measurements of suspension melting temperatures to
describe metastable zone. Phase transformation temperatures have been measured to find the temperatures at which consolidation start. For this express purpose has been utilized thermocouples Typ K NiCrNi (ZA9020-FS Ahlborn) and data logger ALMEMO 8990-8 (Ahlborn) connected with computer
The majority of the experiments in this study were conducted using the illustrated (in Chapters 3.1 and 3.2) experimental setups. In this chapter, the results of
measurements and tests will be given. The presentation of results for various suspension densities and operating temperatures and their relationship with the major properties in focus (overall porosity and pore size distribution) will follow. Chapter 4.1 deals with rheological properties of the used suspensions. In Chapter 4.2 data of the ice crystallization process will be given. Finally, the investigations on the overall porosity and pore size distribution are presented in Chapter 4.3.
The rheological properties of suspensions are extremely important for the processing. The particle size distribution, interparticle forces and solid filler content can in close relation to their temperature dependence determine those properties. In this chapter density and viscosity measurements of investigated ceramic suspensions (see Chapter 3.1) will be presented.
The slurry densities have been investigated in a temperature range of 5 to 25°C. Temperatures below 0°C has not been examined because a potential freezing of the water and thereby the volume expansion might damage the device. The relative density measurements are shown in Fig. 5-1. The relative density (RD) is the density of the slurries related to the density of the liquid phase (water). This value is always greater than unity because of the presence of solid particles in the suspension.
phase liquid of density slurry of density RD ⋅ ⋅ ⋅ ⋅ ⋅ = (5.1)
The density is a temperature dependent function therefore it needs to be reported at exact temperature. The increase of density by decreasing temperature, Fig. 5-1, is related to a density incensement of the liquid phase (water). Density changes due to temperature of the solid particles in this temperature region are insignificant and can
From Fig. 5-1 it is obvious that an increase of the density depends on the solid loading. Higher solid loads correspond to less water in the slurries and therefore an increasing of the slurry density.
Temperature [°C] 0 10 20 30 Slurries den sity [g /cm 3 ] 1,2 1,4 1,6 1,8 2,0 2,2
2,4 46 Vol.% Solids40 Vol.% Solids
36 Vol.% Solids 32 Vol.% Solids 28 Vol.% Solids
Fig. 5-1: Slurries density measurement
The maximal amount of solid in the slurries was 46 Vol.%. A further increase of the solid load has not been reported because the slurries become too dense and not castable any more. Increasing the solid load leads to a formation of high-density zones and agglomerates. Such zones do not allow the ice crystals to grow continuously during freezing and results in microstructural evolution of the final samples.
The effect of increasing density on the microstructural evolution on the final samples is shown in Fig. 5-2. In Fig. 5-2 the freezing temperature and the distance from the cooling plate is the same for all samples. The increase of solid loads will decrease the final porosity of the samples and therefore will have an effect on the mechanical properties of the sample.
Fig. 5-2: Microstructure evolution of slurries with different solid loads (a) 46 (b) 40 and (c) 36 Vol.%
The viscosity is one of the most important factors in the freeze casting process. The temperature dependence of the viscosity strongly effects the suspension quality and the time required for the homogenisation as well as the required cooling rate.
Therefore temperature and solid content dependence have been exanimate. Suspensions were prepared according to the procedure described in Chapter 3.1. The measurements were performed over a wide range of share rates (between 10 to 1000 s-1). The temperature effect was observed in the range of 5 to 25°C by
connecting the beaker of the device with the thermostat and so allowing an adjustment of wanted temperature.
The relations between share rate and share stress are shown in Fig. 5-3.
The slurries with 46 and 40 Vol. % solids display an orderly share thinning behaviour observed with a small yield stress from the hysteresis between ascending and descending curves. With decreasing solid load content share thinning is decreasing this effect as is also reported by Zhu [Zhu02] and Rao [Ram99]. At 28 Vol.% the share rate is almost proportional to the share stress. This slurry exhibits almost Newtonian behaviour (which can be observed from Fig. 5-4) with only a small
deviation at small share rates. The change in suspension behaviour is clearly related to the volume fraction of the solids. In case of high solid loads and low share rates the particles form big agglomerates. Therefore their mobility becomes limited. An increase in share rate affects the suspension structure. A beginning in breaking agglomerates and big particles due to increasing viscosity forces results in only a small deviation in viscosity.
1mm 1mm 1mm
1mm 1mm 1mm
Share rate [s-1] 0 200 400 600 800 1000 1200 Vi scosi ty [mP a. s] 0 20 40 60 80 100 120 140 160 180 200 46 Vol.% Solids 40 Vol.% Solids 36 Vol.% Solids 32 Vol.% Solids 28 Vol.% Solids Share rate [s-1] 0 200 400 600 800 1000 Sh ar e st ress [ P a] 0 20 40 60 80 100 120 46 Vol.% Solids 40 Vol.% Solids 36 Vol.% Solids 32 Vol.% Solids 28 Vol.% Solids
Fig. 5-3: Share rate versus share stress of slurries with various solid contents at 10°C
Fig. 5-5 shows the viscosity dependence on temperature. The data show obviously that with decreasing temperature viscosity increases. This can be explained by a decrease in viscosity of the liquid medium and decreasing of Brownian movement of ceramic particles. By reducing Brownian movement of the particles the forces avoiding agglomerates formation become smaller.
Share rate [1/s] 0 200 400 600 800 1000 Vi sc os ity
η[mPas] 0 20 40 60 80 100 120 140 160 180 200 220 240 5°C 10°C 15°C 20°C 25°C
Fig. 5-5: Viscosity temperature dependence for slurries with 46 Vol.% solid loads at various temperatures
For the shown experimental data the best regression was obtain by using Cross’s model [Cro65]. p s b . 0 1 1 ξ η η η η + = − − ∞ ∞ (5.2)
In this model η0 is a low share viscosity, η∞ is a high share viscosity, b and p are
constants. The constant p has a recommended value of 2/3. ηs is the suspension
viscosity at a specific share rate. The common way to express the suspension viscosity η is to present it as a relative viscosity which is defined as:
η = (5.3)
were ηr is the relative viscosity and ηl is the viscosity of the liquid phase.
Table 5.1: Fitting parameters obtained from the Cross regression for steady share rates of Fig. 5-3 Volume Fraction [Vol.%] η∞ b p R2 0,46 105,3 0,9195 2/3 0,9986 0,40 41,3 0,6761 2/3 0,9997 0,36 20,7 0,3328 2/3 0,9825 0,32 8,1 0,0775 2/3 0,9897
The data for 0,28 Vol.% is not included in Table 5.1 because the slurry does not sufficiently behave like a concentrated suspension and exhibits almost Newtonian behaviour.
Fig. 5-6 shows the extrapolated values of the viscosity calculated by Cross’s
regression. The relative viscosity data are plotted as a function of the volume fraction of solids. The best fit of the data was obtained using the modified Krieger-Dougherty model [Kri59]. n sl sl sr − ⎟⎟ ⎠ ⎞ ⎜⎜ ⎝ ⎛ − = 1 * φ φ η (5.4)
were ηsr is the highest share rate viscosity, φsl is the volume fraction of solids, φ*sl and
n are fitting parameters. In this Figure 5-6 the relative high share viscosity is defined as η∞ from the Cross model normalized by the viscosity of the slurry with no solids
(water in this case 1mPa.s at 25°C), as a function of the volume fraction of solids. The fitting parameter φ*sl shows the maximum volume fraction of solids were the
slurry becomes infinite [Ara04]. The Krieger-Dougherty model yields a maximum solid volume fraction of φ*sl=0,66 suggesting that higher solids volume fractions should
also be attainable for such a complex suspension. On the other hand the value of 0,66 Vol.% was found to be too high because already at ambient conditions in case of solid contents higher than 48 Vol.% a very fast gelation was found and the suspensions could not be handled anymore. Since it is not known how much water molecules still remain in the slurry, compared with those absorbed on the hydrophilic alumina and silica particles surfaces.
Volume fraction of solids
0,0 0,2 0,4 0,6 0,8 R elat iv e high sh are vi sco sity 0 50 100 150 200 250 φm=0,66 n=3,9227 R=0,99748
5.2 Nucleation and Crystal growth
In this chapter the experiments are presented which are carried out on crystallization of ice. The experimental work is divided into two parts. The first set of data is on nucleation. The second part deals with crystal growth.
22.214.171.124 Roughness of the cooling plates
Two different materials, stainless steel and cooper, have been chosen to prepare the cooling plates in the device presented in Fig 3-2. These materials have been chosen because of their mechanical and thermal properties and their wide application in industry. For each material two plates with different roughness have been tested to observe their effects and influences on interfacial tension compared to ceramic suspensions. Haasner [Haa02] has found a correlation between initial roughness and the control of nucleation conditions.
The data obtained and evaluated are plotted in Fig. 5-7. A perthometer technique was used for the roughness measurements. The instrument was equipped with a diamante needle with a radius of 0,25 mm tip. The needle was driven on the plate surface tracking 2 cm. The needle top follows 2 dimensionally the plate topography and the data are recorded into the device memory. Each measurement has been repeated 4 times and is presented as averaged result. From the measurements following parameters have been achieved: Rz andRa. The parameter Rz is an
averaged roughness depth value from the single measuring sections and Ra is the
arithmetic average value of the roughness profile.
The average roughness profile of the used plates was found to be between 0,5 to 0,95µm. The “cooper polished” surface shows a very fine structure. However, some scratches and slits have been detected and they can be seen in Fig. 5-8 (SEM micrographs of the plates). The roughest surface was from the “cooper rough” plate were the depth of the scratches was about 7± 0,29µm. An increasing in roughness profile results in the contact angle and area between suspension and plate because the thermal conduction occurs only through contact regions. In the case of thermal conduction, for example, the roughness can cause distortion in the heat flux but also promote nucleation because of the irregularities.
Cooper polished Cooper rough Steel polished Steel rough Ra [ µm] 0,0 0,2 0,4 0,6 0,8 1,0 Rz [ µm] 0 2 4 6 8 10 Ra Rz
Fig. 5-7: Measurements of the roughness profiles
126.96.36.199 Contact angle
When the liquid is placed on a solid substrate it will wet the surface to a certain degree, therefore droplets with different forms and profiles are formed depending on both the interfacial tension and the contact angle.
The micrographs from the droplet profiles have been recorded by a CCD camera and a microscope connected with a computer. The micrographs have been evaluated using the contact angle measurement device software. In order to separate the droplet profiles from the environment a back light source was used.
A schematic view of the measurement device is shown in Fig. 5-9.
To put droplets on the substrate surface a syringe with a micrometer piston has been used. Such syringe was used in order to control the droplets volume. All presented experiments have been carried out with droplets with a size of 3± 0,1mm.
The solid substrate surface was the cooling cell surface, which is in contact with the ceramic slurries to be frozen, as shown in Fig. 3-2. The cooling cell was connected with a thermostat allowing setting the desired temperatures. All investigated suspensions were in the temperature range between +5 and -30°C.
Fig. 5-9: Schematic view of the contact angle measurement system
First the syringe needle was placed as close as possible to the solid substrate surface. After the droplet was formed it was removed. The micrographs have been taken immediately after the syringe needle was removed. That avoiding to gain measurement mistakes of the droplet profiles in dependence with time. Before starting the measurements the used surface was carefully cleaned in order to
Flow direction Computer Cooling cell Cooling liquid Microscope and CCD camera Sirynge with micrometer piston Back light Flow direction Computer Cooling cell Cooling liquid Microscope and CCD camera Sirynge with micrometer piston Back light
diminish results on the contact angle values from inhomogeneities and impurities on the solid substrate surface.
In Fig. 5-10 are micrographs shown of the droplets profiles.
In Fig. 5-11 are the measurement results plotted of investigations on the contact angle in dependence of the substrate surface temperature. For all presented data the substrate was used is a “steel rough” surface. An increase in contact angle results in a decrease in temperature. At least 5 measurements were taken for each pair suspension/substrate surface in order to obtain average values. All presented data show such an average value for the contact angle.
Fig. 5-10: Droplets profiles. Micrographs taken on “Steel polished” surface for 36 Vol.% solid load
From the data in Fig. 5-11 it can clearly be seen that the non-wetting behaviour of suspensions on the steel surface is increasing with decreasing temperature. The data of the other surfaces are shown in Appendix A. (The found behaviour is in principle the same as presented above). Figure 5-12 illustrates the contact angle measurements for suspension drops impacted onto the stainless steel or the cooper surfaces. Figure 5-12 evidently demonstrates that the contact angle is a direct correlation of the pair liquid substrate surface. The variations of the contact angle values have been found significant by varying the substrate material, which can be connected to differences in interfacial tension values. The substrate surface roughness has been found to have little influence on the contact angle in the range of the experimental settings. For example at –20°C for suspensions with 40 Vol.% solid load the difference of contact angle between steel rough and the polished surface is 1,2° which lies in the error range of the measurement.
Temperature [°C] -35 -30 -25 -20 -15 -10 -5 0 Contac t angle [degree] 40 60 80 100 120 140 46 Vol.%40 Vol.% 36 Vol.% 32 Vol.% 28 Vol.%
Fig. 5-11: Effect of temperature on contact angle. Measurements of a steel polished surface
Fig. 5-12: Effect of substrate material and roughness on the contact angle for suspensions with 40 Vol.% solid load
Cooper-roughCooper-polished Steel-rough Steel-polished
Contact angle [de
g ree ] 60 70 80 90 100 110 Temperature -10°C Temperature -20°C
188.8.131.52 Surface tension of suspensions
A Drop Shape Analysis System (DSA) was used to measure the surface tension. A chamber for temperature control was used. Two opposed walls of the chamber were made of glass. The temperature chamber was connected with a thermostat allowing adjustments of the desired temperature. The suspensions were put into the temperature chamber by using a syringe with a micrometer piston. A controlled volume of the suspension droplets was achieved by slowly moving the syringe piston to form a pendant drop hanged on the syringe needle. The syringe and the temperature chamber were placed in such a way that on the one side was a light source and on the other side a CCD camera and a microscope. The microscope was connected with a computer, which allows viewing the droplet profile on-line, recording the pictures and making those available for evaluations by using appropriate software. The formed droplets have different profiles in dependence of solid load content or temperature. The profile is a result of a reached equilibrium between droplet surface forces and its environment, respectively, (in presented data) and the gravitation forces. Drop profiles were recorded and evaluations over time intervals of 0,5 to 60s were carried out. The characteristic suspension densities obtained from density measurements (presented in Chapter 4.1.1) were entered into the software and the surface tension values were determined by analysis based on the Wu [Wu71, Wu82] and the Zisman [Zis64] technique.
The data obtained for suspension surface tensions versus temperature are plotted in Fig. 5-13.
The plot shows that with decreasing temperature the surface tension is slightly increasing. The experimental procedure was repeated at least 20 times and averaged results are presented.
The surface tension has been investigated in a temperature region between 0 and 20°C. Measurements for temperatures below 0°C have not been carried out because the suspensions start to freeze.
The surface tension has increased with increasing solid load content, which shows on the one hand that the ceramic particles become more surface active in aqueous suspension and the interactions between water molecules and ceramic particles is very strong. On the other hand the surface tension increases at high solid concentrations are less pronounced.